THE CHARACTERIZATION OF BONDED PHASES FOR HIGH PERFORMANCE LIQUID CHROMATOGRAPHY
Item Type text; Dissertation-Reproduction (electronic) Authors Stetzenbach, Klaus John
Publisher The University of Arizona.
Rights Copyright © is held by the author. Digital access to this material is made possible by the University Libraries, University of Arizona.
Further transmission, reproduction or presentation (such as public display or performance) of protected items is prohibited except with permission of the author.
Download date 28/06/2022 22:56:27
Link to Item http://hdl.handle.net/10150/282293
INFORMATION TO USERS
This was produced from a copy of a document sent to us for microfilming. While the most advanced technological means to photograph and reproduce this document have been used, the quality is heavily dependent upon the quality of the material submitted.
The following explanation of techniques is provided to help you understand markings or notations which may appear on this reproduction.
1. The sign or "target" for pages apparently lacking from the document photographed is "Missing Page(s)". If it was possible to obtain the missing page(s) or section, they are spliced into the film along with adjacent pages.
This may have necessitated cutting through an image and duplicating adjacent pages to assure you of complete continuity.
2. When an image on the film is obliterated with a round black mark it is an indication that the film inspector noticed either blurred copy because of movement during exposure, or duplicate copy. Unless we meant to delete copyrighted materials that should not have been filmed, you will find a good image of the page in the adjacent frame.
3. When a map, drawing or chart, etc., is part of the material being photo
graphed the photographer has followed a definite method in "sectioning"
the material. It is customary to begin filming at the upper left hand corner of a large sheet and to continue from left to right in equal sections with small overlaps. If necessary, sectioning is continued again—beginning below the first row and continuing on until complete.
4. For any illustrations that cannot be reproduced satisfactorily by xerography, photographic prints can be purchased at additional cost and tipped into your xerographic copy. Requests can be made to our Dissertations Customer Services Department.
5. Some pages in any document may have indistinct print. In all cases we have filmed the best available copy.
300 N. ZEEB ROAD, A NN ARBOR, M l 48106 18 BEDFORD ROW, LONDON WCIR 4EJ, ENGLAND
STETZENBACH, KLAUS JOHN
THE CHARACTERIZATION OF BONDED PHASES FOR HIGH PERFORMANCE LIQUID CHROMATOGRAPHY
The University of Arizona PH.D. 1980
International300 N. Zeeb Road, Ann Arbor, MI 48106 18 Bedford Row, London WCIR 4EI, England
THE CHARACTERIZATION OF BONDED PHASES FOR HIGH PERFORMANCE LIQUID CHROMATOGRAPHY
Klaus John Stetzenbach
A dissertation Submitted to the Faculty of the DEPARTMENT OF CHEMISTRY
In Partial Fulfillment of the Requirements For the Degree of
DOCTOR OF PHILOSOPHY In the Graduate College THE UNIVERSITY OF ARIZONA
1 9 8 0
THE UNIVERSITY OF ARIZONA GRADUATE COLLEGE
As members of the Final Examination Coiranittee, we certify that we have read
the dissertation prepared by Klaus John Stetzenbach
entitled The Characterization of Bonded Phases for High Performance Liquid Chromatography
and reccmmend that it be accepted as fulfilling the dissertation requirement
for the Degree of Doctor of Philosophy .
Final approval and acceptance of this dissertation is contingent upon the candidate's submission of the final copy of the dissertation to the Graduate College.
I hereby certify that I have read this dissertation prepared under my direction and recommend that it be accepted as fulfilling the dissertation requirement.
STATEMENT BY AUTHOR
This dissertation has been submitted in partial fulfillment of requirements for an advanced degree at The University of Arizona and is deposited in the University Library to be made available to bor
rowers under rules of the Library.
Brief quotations from this dissertation are allowable without special permission, provided that accurate acknowledgment of source is made. Requests for permission for extended quotation from or re
production of this manuscript in whole or in part may be granted by the head of the major department or the Dean of the Graduate College when in his judgment the proposed use of the material is in the in
terests of scholarship. In all other instances, however, permission must be obtained from the author.
for her patience, support and love
The author wishes to express his sincere gratitude to Dr.
Michael F. Burke for his encouragement, guidance and support during the course of this study and in the preparation of this manuscript.
The author would like to thank Dr. Dean Carter of the Toxicology Program for providing equipment throughout the course of this study.
The author also wishes to thank Dr. George Wilson for his thorough review of this manuscript.
The author would also like to thank the faculty and students of The Department of Chemistry for their assistance and encouragement.
TABLE OF CONTENTS
LIST OF ILLUSTRATIONS vii
LIST OF TABLES ix
1. INTRODUCTION 1
Grignard Reactions 11
Silane Reactions 12
Chromatographic Experiments 24
Peak Position 25
Peak Broadening 27
Non-Chromatographic Experiments 30
Batch Extraction Experiments 31
2. PROCEDURES 32
Materials and Reagents 32
Modification Procedures 33
Silanization Reactions 33
Amide Reaction 35
Grignard Reactions 35
Column Packing Procedure 37
Methyl Red Experiment 39
NMR Experiments 40
Batch Extraction Experiments 40
Liquid Chromatographic Experiments 41
Elemental Analysis 42
Bonded Phases Studied 43
Physical Considerations of the Bonded Phases 47 3. NON-CHROMATOGRAPHIC EXPERIMENTAL RESULTS 48
Methyl Red 48
Solvent Extraction 50
^^C NMR Experimental Results 55
vi TABLE OF CONTENTS—Continued
4. CHROMATOGRAPHIC RESULTS 70
Capacity Factor Considerations 72
AH Considerations 74
Non-specific Interacting Solutes . 74
Free Energy Considerations 82
Entropy Considerations 83
Specific Interacting Molecules 85
5. BAND SPREADING 90
6. CONCLUSIONS AND SUGGESTIONS FOR FUTURE WORK 99 APPENDIX 1: CHROMATOGRAPHIC RETENTION DATA 102
APPENDIX 2: AH VALUES 119
APPENDIX 3: AAG' VALUES 124
APPENDIX 4: AAS' VALUES 132
APPENDIX 5: THEORETICAL PLATE MEASUREMENTS 141
APPENDIX 6: RETENTION ERRORS 152
LIST OF ILLUSTRATIONS
1.1. Pore structure of a totally porous silica particle 4
1.2. Chemical structure of silica 7
1.3. Possible terminal hydroxyl configuration of silica 7 1.4. Dichlorodimethyl silane modified silica 8 1.5. Monofunctional organosilane bonded to a silica surface ... 16 1.6. Possible configurations of organic phase bonded to silica
when a polyfunctional reagent is used 17 1.7. Inter- and intra-chain interactions of the bonded phases . . 18 1.8. Bonded phase solvated by the organic modifier . 19 1.9. Bonded phase solvated by a stagnant layer of mobile
2.1. Apparatus for drying silica beads 36
3.1. Structure of methyl red 49
3.2. 13 C NMR spectrum of 10% ODS modified silica in
3.3. NMR spectrum of 10% ODS 60
3.4. 13 C NMR spectrum of 5% ODS in methanol 62 3.5. 13 C NMR spectrum of 10% ODS in methanol 63 3.6. 13 C NMR spectrum of 20% ODS in dioxane 64
3.7. NMR spectrum of 10% ODS in 50/50 methanol/D20 65 3.8. 13 C NMR spectrum of RP-8 in 50/50 acetonitrile/D^O 68
4.1. Plots of In k' vs 1/T for 5% ODS and RP-8 bonded phases . . 76 4.2. Plots of In k' vs 1/T for 20% ODS bonded phase with
methanol and THF used as organic modifiers 77 vii
viii LIST OF ILLUSTRATIONS—Continued
4.3. Plots of In k' vs 1/T for 10% ODS and amide bonded
4.4. Plots of In k' vs 1/T for aniline 87
5.1. Plot of HETP (H) vs linear velocity (y) for benzene and
isopropyl benzene on the 10% ODS bonded phase 95 5.2. Plot of HETP (H) vs linear velocity (p) for benzene and
isopropyl benzene on the 20% ODS bonded phase 96 5.3. Plot of HETP (H) vs linear velocity (y) for benzene and
isopropyl benzene on the 5% ODS bonded phase 97
LIST OF TABLES
2.1. Bonded phase specifications 34
2.2. Bonded phases prepared by Grignard reactions 38 3.1. Results of the methyl red experiments 49 3.2. Results of the heptane solvent extraction experiments ... 51 3.3. Amount of organic modifier adsorbed by the bonded
3.4. 13 C NMR chemical shift and line width data for octa-
decane and octadecyl modified silica 57 3.5. 13 C NMR chemical shift data for octane and the RP-8
bonded phase 67
4.1. The solvent strength of some water/methanol and water/
THF mobile phases 71
4.2. The retention of benzene, toluene and naphthalene in
water/methane/hexane compared to water/methanol .... 85
The physical and chemical nature of chemically bonded phases used in high performance liquid chromatography have been studied. These bonded phases were characterized by a variety of chromatographic and non-chromatographic experiments. The non-chromatographic techniques included 13 C NMR and batch extraction methods. The role played by the
bonded phase as well as the mobile phase in determining the retention characteristics of the "stationary phase" were determined.
The retention of solute molecules on bonded phases was found to be a function of the chain length of the bonded phase, the chemical nature of the bonded molecule, and the type of organic modifier used in the mobile phase. The energetics of the solute-stationary phase inter
actions was determined by the differential enthalpy and was found to be indicative of a partitioning process between two liquid phases.
The retention process was also affected by the surface coverage of the bonded molecule. Optimum retention and separation characteristics were obtained with a hydrocarbon bonded phase of high surface coverage when used with a mobile phase containing a very polar organic modifier.
The efficiency of these bonded phases was found to be indepen
dent of chain length as well as surface coverage of the bonded molecule.
Some bonded phases which have specific functionalities incorporated into the bonded molecule are not true reversed phases.
The selectivity of the bonded phases towards polar solute mol
ecules was found to be affected by the t3T)e of organic modifier used in the mobile phase.
The major accomplishment of this work shows that the stationary phase consists of the bonded molecule as well as trapped mobile phase.
The composition of this ternary mixture is a function of the type and amount of bonded material and the type and amoxmt of organic modifier used in the mobile phase.
Chromatographic separation techniques represent some of the most powerful tools available to the scientist today. A better understanding of the processes which are responsible for the selectivity and efficiency of currently available stationary phases for use in gas and liquid
chromatography is necessary if we are to develop stationary phases which will be appropriate for the separations problems of the future.
In order to contribute to the improvement of chromatographic systems it is necessary to understand the progress which has been made in the last twenty years. In a chromatographic system the sample components are distributed between the mobile phase and the stationary phase. Since all the sample molecules are introduced into the system at essentially the same time, the components must migrate through the column at
different rates to separate from each other. This differential migra
tion process is dependent upon a driving force and a retarding medium.
The rate of migration is determined by the fraction of time that the solutes spend in the mobile phase versus the time spent in the sta
tionary phase. The fraction of time it spends in the mobile phase, and therefore moving at the rate of the mobile phase, is a function of the relative affinity that the sample molecules have for each of the two immiscible phases. The amount of mobile phase that is required to
2 elute the solute to the peak maximum is a measure of the affinity that the solute has for the stationary phase.
The transfer of the solute between the two phases must also be done efficiently. As soon as the sample molecules are introduced onto the column they begin to spread. In order to achieve baseline resolu
tion one component must be completely eluted before the next component starts to elute. Narrower bands allow the peak positions of the components to be closer. This not only decreases the time of the experiment but it also improves the detection limit. High efficiency requires rapid transfer of the solute molecule between the mobile and the stationary phase. The efficiency can be enhanced by the use of stationary phases with small particle diameters, uniform pore size and high surface area. The selectivity of the stationary phase can be modified through the coating or bonding of other molecules to the surface.
In liquid chromatography the mobile phase is a liquid or a mixture of miscible liquids. The choice of the composition of the mobile phase to provide the driving force is dependent upon the stationary phase and the solubility of the sample components. The retarding mechanism can be an adsorption on the solid surface of the stationary phase or it can be a liquid-liquid partitioning if the solid support has been modified by coating it with an immiscible liquid or by chemically derivatizing the surface. Separations can also be achieved by taking advantage of large size differences in the solute molecules. The most useful stationary phase for liquid-liquid
3 partitioning would be a truly stationary liquid and for adsorption a specifically tailored surface. Since no two liquids are completely immiscible and adsorbent surfaces require modification the most
promising approach appears to be the use of chemically bonded materials.
An ideal support for liquid chromatography has to have good mechanical stability to withstand the high pressure drop due to the small particles. It should be inert and have a very high surface area.
This means the particles must be porous and these pores should also be uniform in size. Uniformity in particle size and shape will greatly improve the packing efficiency. Liquid chromatography support materials have been made of silica as well as alumina and carbon. Because of the high activity and catalytic properties of carbon and alumina, silica has become the most widely used chromatographic support material.
Although silica particles have large surface areas and good mechanical stability, the uniformity of size and shape and the pore structure are not ideal. Figure 1-1 shows a typical porous silica. Variations in pore size may possibly lead to exclusion of some molecules. The surface of the silica contains hydroxyl groups, separations on unmodified silica depend upon the interactions of the solute molecule with these surface groups. These hydroxyls also serve as points of attachment for the bonded molecules. The silica can be modified by reacting an alkyl- silane, usually octadecyltrichlorosilane with the surface hydroxyl.
(The reactions will be discussed in detail later.)
Chemically bonded stationary phases have been one of the more important contributing factors to the advancement and great popularity that has been achieved by modern liquid chromatography. Advances in
POROUS SILICA PARTICLE
Figure 1.1. Pore structure of a totally porous silica particle
5 this area have been reviewed in several recent articles (1-4). The advantages of reversed-phase^ chemically bonded liquid chromatography over conventional liquid-liquid chromatography have also been dis
cussed (6). Most modem chemically bonded phases have a hydrocarbon such as octadecane bonded to the silica as a stationary phase and use a mobile phase consisting of water modified by a water miscible organic solvent such as methanol, acetonitrile or tetrahydrofuran. Although 70-80% of all liquid chromatography is done on chemically bonded phases, the retention mechanisms are not completely understood. Knowledge of the retention mechanism of a solute will allow more accurate prediction of specific separation conditions. It will also help in preventing the spread of specialty application stationary phases such as has happened in gas-liquid chromatography. With a good understanding of the reten
tion mechanism, only a few stationary phases are necessary because of the ability to manipulate the mobile phase (7).
Attempts to determine retention mechanisms in liquid chroma
tography have been undertaken by a number of workers (2,8,9). Most of these attempts have used only changes in mobile phase and solute molecules to characterize the retention mechanism. It is usually assumed that these changes do not affect the chemical or physical nature of the stationary phase, and that the retention is determined solely by the chemical composition of the mobile phase. The most common current approach involves assuming the water present in the
1. The term reversed-phase was first used by Martin and Synge (5) to describe a form of liquid-liquid chromatography in which the
mobile phase was more polar than the stationary phase.
6 mobile results in a hydrophobic effect which forces the solute molecule into the stationary phase (10). The stationary phase is thought to be merely a passive receptor for the solute molecules. It has been known for years that silica gel can be modified by certain mobile phase
solvents (11). Work in this laboratory has shown that a mobile phase of 0.67 methanol in chloroform was able to separate a mixture of four aflatoxins on silica gel while the same components could not be eluted with pure chloroform. Since the solvent strength of both solvent sys
tems is essentially the same as that of chloroform, it must have been modification of the silica by the methanol that affected the separation.
If silica can be modified by the mobile phase then one might also sus
pect the same is true of chemically bonded phases. To believe that the chemically bonded phase merely acts as a passive acceptor for the solute molecule when it is forced from the mobile phase is to completely shut out the thought of any mobile phase-stationary phase interactions. The hydrophobic chromatography theory fails to recognize that these inter
actions exist. To have a more complete understanding of these in interactions we must have a complete chemical and physical description of the parei.' silica gel and the organic molecules that are bonded to them.
Porous silica materials have an internal structure that is produced by the bonding of a silicon atom to four oxygen atoms and each oxygen atom is bound to two silicon atoms, which results in an empirical formula of (SiO„) (Fig. 1.2). On the surface the terminal silicon atoms
have hydroxyl groups bonded to them. There are several possible con
figurations for these hydroxy groups (Fig. 1.3).
Figure 1.2. Chemical structure of silica
OH OH 1 1
1 0'- 0
HO-Si-O-Si-OH -O-Si-0--Si- 1 1
-Si-O-Si- -Si-O-Si- HO-Si-OH
1 1 1 t 1
-Si-O-Si- 1 1 0
0 0 0
1 0 t 1
1 1 -Si-0--Si- 1
(a) ' 1
(b) (c) (d) (e)
Figure 1-3. Possible terminal hydroxyl configuration of silica
It is also possible that siloxane bridges terminate the silica structure (Fig. 1.3 e). Figure 1.3 c and d are structurally equivalent. The dotted
line in Figure 1.3 d indicates the possibility of hydrogen bonding between neighboring hydroxyl groups. Physically adsorbed water is also present on the silica surface unless it has been heated to extremely high temperatures (12)•
Snyder and Ward (13) believe the surface to consist of all the possible configurations shown in Figure 1.3 a-e, depending upon structural considerations. Gilpin and Burke (14) through their work with
bonding mono- and dichlorosilanes to Porasil have come to the conclusion (D
that each surface silica atom has only one terminal hydroxy group, and that these hydroxyl groups condense to form siloxane bridges, only upon heating to about 600°C. Peri (15,16) believes the surface to be made up
geminal hydroxyl groups (Fig. 1.3 b). Unger and Gallei (.17) have shoxm
8 that silica chlorinated with silicon-tetrachloride, as shown in Rx-1, upon hydrolysis never has a larger OH content than the unreacted product.
Si-OH + SiCl, > Si-OSiCl„ + HCl Rx-1
This indicates that the OH groups on neighboring silicon atoms must condense to form siloxane bonds, leaving only one terminal hydroxyl group. However, in his reactions with organolithium compounds (Rx-2) on chlorinated silica gel (18) siloxane bridging after hydrolysis was not observed,. This was believed to be due to steric hindrance by the large organic molecules.
Si-0-SiCl_ + LiR > Si-O-Si-R R = 0, 0,, 0, Rx-2
J I ^ ^
When Gilpin ( 19 ) reacted dichloromethyl silane with Porasil and hydro- lized the remaining chlorine he describes a structure as shown in
Fig. 4, indicating that the majority of the remaining hydroxyls condensed to form siloxane bonds.
I 3 » 3 CH,-Si-0-Si-CH-
3 I I 3 0 0
-Si-O-Si- I I
Figure 1,4. Dichlorodimethyl silane modified silica
The conclusions of these experimental results are that there are no significant amounts of surface groups other than those described by Figure 1.3 c and d. If poly-functional silanes are used to
9 modify silica it is possible for them to form a polymeric network like that of the parent silica gel. If there is steric hindrance from the organic portion of the molecule the polymer will not form, but there will always be less than two bonds to the surface.(20).
If one assumes the surface of the silica to be made up of a monolayer of hydroxyl groups the question then arises as to how
many of these there are in a specific area. This is important because estimates of bonded phase densities will have to be calculated with this value. Iler (21) and Kiselev (22 ) conclude that there are eight hydroxyls per 100 A on a fully hydrated surface. Other researchers 02
(16,18) have put the number at five hydroxyl groups per 100 A . This number may be as low as 20H/100 A depending upon the type of silica 02 and its previous treatments (16). Four to five hydroxyls/100 A is °2
considered to be the characteristic concentration for the type of silica commonly used in chromatographic studies ( 23). This allows an average surface area of 20 to 25 A per OH group, or an average distance 02 of approximately 5 A between OH centers. o
These silanol groups are weakly acidic and can be titrated in a concentrated NaCl solution with NaOH (24). However, this method cannot be used to determine a specific surface area by assuming four hydroxyl
groups per 100 A because the individual beads are made up of aggregates, of smaller ones which are held together by siloxane bridges that
dissolve in basic pH and produce two silanol groups. The number of OH groups titrated therefore is considerably larger than those available for modification or surface area measurements.
10 It has also been suggested that thionyl chloride can be used for the determination of surface hydroxyl groups on silica if the pore size is not very narrow (25;. Pores narrow enough to exclude SOCI2 would almost certainly also exclude most solute molecules and all presently used organic modifying reagents used in making reversed phase column packing materials. Thionyl chloride reacts with silanol groups (Rx-3) in a 1:1 ratio,
SiOH + SOCI2 > Si-Cl + SO2 + HCl (Rx-3)
so that each accessible hydroxyl group is replaced with a chlorine.
Since the Si-Cl bond is easily hydrolized, the CI can be removed and determined through titration with silver nitrate (18). In this way, the number of accessible surface hydroxyl groups can be determined.
However, work done in this laboratory and by others (26,27) using thionyl chloride and Grignards to modify silica have produced bonded phases with very low percentages of carbon. This is attributed to the poor initial chlorination of the silica by thionyl chloride. If the reaction does not go to completion then numbers obtained from such an experiment are not an absolute measure of the surfact area but only a measure of the surface area available to thionyl chloride which may not be the same as the surface area available to a solute molecule.
The first chemically bonded organic stationary phases used in liquid and gas chromatography were made by the esterification of porous glass and aliphatic alcohols (28). These silicate esters which have Si-O-R bonds are not very thermally nor hydrolytically stable (29),
which severely limits the usefulness of this tjrpe of bonded phase as a reversed-phase stationary phase. A direct silicon carbon bond (Si-C) is considerably more stable than the Si-O-C bond. There is evidence that it is even more stable than the Si-O-Si bond (26). The stability of silica gel arises from its polymeric structure, not the strength of an individual silicon-oxygen bond. Two reactions produce bonded phases that have silicon-»carbon bonds. These are discussed in detail below.
Grignard reactions with chlorosilanes have been known for some time (30). Deuel and Wartmann state that they were the first to use this reaction to derivatize silica gel in 1958 (26). The first to employ these preparations on substrates used for liquid chromatography were Locke, Schmermund and Banner in 1971 (27). . Their work,
unfortunately, is vague and very little chromatographic data is presented. The advantage of the Grignard reaction is that it forms a single bond between the bonding molecule and the silica if thionyl chloride is used to chlorinate the silica. The silicon atom that forms the bond is from the silica gel matrix. It is bonded to three other silicon atoms through the siloxane linkages, making this the most stable of the non-polymeric bonded phases.
The first step in the preparation of a bonded phase with a Grignard reaction is to thoroughly dry the silica to remove all water, without condensing the surface hydroxyls. 150° C has been suggested as the most appropriate temperature (19). The water not only deacti
vates the Grignard but it can also hydrolyze the silicon chlorine bond.
12 Chlorination of the silica can be accomplished through Rx-1 or Ey-3. It would appear that SiCl^ should be a more efficient chlorinating agent than SOCI2 but Unger et al. ( 18 ) found that the amount of CI on the surface on several silica gels that had been reacted with SiCl^ or SOCI2 had a ratio of about 2:1, not 3:1 as expected. This was
attributed to steric exclusion of the larger SiCl^, but it could also be that hydrolysis, because the silica cannot be completely dehydrated, and the formation of siloxane bridges caused the unexpected ratio.
From experiments done for this work and by others there, appears to be no significant difference in the chlorination efficiency of SOCI2 and SiCl^. They react with about 80% of the available surface silanols (31). Thionyl chloride appears to be the reagent of choice because it does not introduce any additional silanol groups (see above).
Although the Grignard reaction modification method should work very well, most workers (including attempts to prepare bonded phases
by this method for this work) find the amount of material bonded to the surface to be discouragingly low. The amount of carbon by weight usually does not exceed 3%. While these types of phases do exhibit some reversed phase characteristics, they are for all practical purposes only pacified silica gel phases.
According to manufacturer's literature, chlorosilanes are used to make all commercial reversed phase packing materials. One of the earliest descriptions of reactions of these types of compounds was given by Howard and Martin (5 ). Many references exist (32-40 ) for the
13 preparation of organosilane bonded phases. Trichlorosilanes are most frequently used. These react with silanol groups to form an Si-O-Si-C bond (Rx-4).
Si-OH + RSiCl^ > -Si-O-Si-R (Rx-4)
Unger et al. (35) see the formation of multiple bonds between the trichlorosilanes and the surface. The number of bonds is greater than one but less than two. This leads to the conclusion that multihalo silane bonded phases have greater stability since more than one bond must be broken simultaneously to remove the bonded phase. Unger (18) and Burke and Gilpin ( 14 ) have shown that poly-functional reagents can form siloxane bridges upon hydrolysis if there is no stearic hindrance.
This would certainly improve the stability of the bonded phases.
Arkels (41) has suggested that trace amounts of water in the solvent causes the organo-trichlorosilanes to polymerize prior to their reac
tion with the silica gel. This would produce a polymeric type coating with a large number of bonds to the surface, thereby producing a very stable bonded phase. This type of mechanism is thought to occur on heavily loaded bonded phases (that use trifunctional reagents). How
ever, this will leave a large number of free hydroxyl groups upon hydrolysis from both the chlorosilane and the silica gel surface.
Scott and Kucera ( 8) have shown that even with these heavily loaded stationary phases hydroxyl groups are still available to interact with solute molecules. Organosilane polymers may be too large to enter all the pores of the silica which can create a large unmodified area or if the pore is blocked by the polymer the surface area of the stationary
14 phase will be reduced significantly. The wet solvent method has also been shoxra to give less reproducible results (42).- Barry (43) has . also suggested that the polymerization occurs on the surface of the silica because of the layers of water that are always associated with silica even when it has been dried at very high temperatures. The :.bonded phase poljrmer may actually be only hydrogen bonded to the hydrated
surface. However, the large number of hydrogen bonds could provide for a very insoluble bonded layer.
Although the possibilities of a dynamic process between the bonded phase and the surface does exist evidence from the use of mono- functional silanes indicates that the bonded phase is fixed to the surface. Monofunctional silanes produce bonded phases of the "brush"
form described by Halasz and Sebastian (28). Because they can only form one bond their stability is decreased at pH greater than 7 (35).
However, the stationary phases made from monofunctional reagents that were used in this work showed no signs of deterioration when used with mobile phase-pH values of 5.5.to 6.0.
Trialkoxy silanes are also employed as reagents in binding organic phases. They are generally less reacti.ve and since they produce no acid upon hydrolysis they may be more convenient to use. Increasing the size of the alkoxy group decreases the rate of hydrolysis ( 41) which may be a useful method for controlling polymerization.
In order to be able to say something about the chemical proper
ties of the bonded phase we must know some of its physical
characteristics. Normally, we describe a compound by its physical
15 properties such as solid, liquid, viscosity, density, etc. These are a all bulk properties and it must be remembered that the bonded phase is one or more layers of hydrocarbon with one end of the molecule held rigidly into place. We must therefore be very careful about comparing the physical properties of the bonded phase with the bulk hydrocarbon.
Of these properties only the average density or spacing between the bonded molecules can be determined providing that an accurate surface area measurement can be made.
With monofunctionally bound phases we know that only one molecule can be bound to one surface hydroxyl (Fig. 1-5) but the regularity of_the spacing (density) may be dependent upon the pore structure of the silica gel. Whenever polyfunctional reagents are used the bonded phase may not be uniform. Both stick and brush like structures (Fig. 1.6) may exist.
Chain length and spacing density will affect molecular interaction
between neighboring molecules or intra-chain interactions (Fig. 1.7). Will the chain stand away from the surface or does it lie down on it?
In liquid chromatography the mobile phase becomes another variable which can affect the stationary phase. The mobile phase may solvate the bonded phase or the silica surface or both. Different components of the mobile phase solvate the organic molecule and the unreached silanols. The hydrocarbon may be surrounded by pure organic modifier from the mobile phase (Fig. 1.8) or there may be a stagnant
layer of mobile phase which is enriched in the organic modifier (Fig. 1.9).
In liquid chromatography the solute molecule is dissolved in and is surrounded by the mobile phase molecules. While it is in this phase it travels at the velocity of the mobile phase. If it never went
H C H
H C H
H C H
H C H
H C H
H C H
H 3 C
S i -
H C H
Figure 1.5. Monofunctional organosilane bonded to a silica surface
Figure 1.6. Possible configurations of organic phase bonded to silica when a polyfunctional reagent is used
Figure 1.7. Inter- and intra-chain interactions of the bonded phase
Figure 1.8. Bonded phase solvated by the organic modifier
B i®® V X®® I ® ® ® ® > ®Vx ^@#®^ X®J®®®x ®
^ ® l v ® ®
X® > ® @ y ® \ ® I ^ ® ® \ ® ® ^ ® ® V ® ® ®
® \ ® ® X @ ®
SOLVATED BONDED STATIONARY PHASE
9. Bonded phase solvated by a stagnant layer of mobile phase
21 into the stationary phase, it would not be retained. So, in order to separate two components they must have different residence times in the stationary phase. To transfer to the stationary phase, a solute
molecule must break its interactions with the mobile phase and form new solvation bonds in the stationary phase. The sum total of this breaking and remaking of bonds and of creating and collapsing cavities in the two p h a s e s i s g i v e n b y t h e f r e e e n e r g y c h a n g e ( A G ) .
The enthalpy change can be considered as a measure of the environmental changes that a solute molecule undergoes in transferring from the mobile to the stationary phase. If this phase transfer
requires the molecule to have a specific orientation or alignment then there will also be a change in entropy (AS). The changes in entropy and enthalpy can be used to calculate the overall change in free energy (AG) of the phase transfer (Eq. 1-1).
AG = AH - TAS (1-1)
These thermodynamic parameters (AG, AH, AS) can be used to provide insight into the mobile phase-stationary phase transfer mechanisms.
However, only AH can be measured accurately from chromatographic data.
The Clausius-Clapeyron equation (Eq. 1-2)
^= =f- (1-2)
K = thermodynamic distribution constant R = gas law constant
T = temperature °K
22 shows that a plot of InK vs will result in a line with a slope of -AH/R. If K is not known the capacity factor (k') can be substituted since k' is proportional to K (Eq. 1-6). The position of the line on the y axis will vary but its slope will be the same.
_ amount of solute in the stationary phase (1-3) amount of solute in the mobile phase
_ R M
where V = retention volume K
= volume of mobile phase required to elute a non- retained solute
_ concentration of solute in the stationary phase concentration of solute in the mobile phase
K = k'(j) (1-6)
<j) = phase ratio
• - J - (1-7)
where Vg = volume of the stationary phase V„ = volume of the mobile phase
Ag = surface area of the stationary phase
If a K value is available then AG can be calculated from Eq.
Eq. (1-8). However, accurate K values can be obtained only when V is known as is the case only in liquid-liquid chromatography or it can be
calculated through the use of solubility parameters (6) (44).
AG = -RTlnK (1-8)
By knowing. 5 values for the solvent, solute and the stationary phase, K can be calculated from Eq. l-^Q.
V.[6.-6 - (6.-6
In K = ^ ^ " i—§_ (1-9)
V. = molar volume of the solute 1
6^ = solubility parameter of the solute 6^ = solubility parameter of the mobile phase 6^ = solubility parameter of the stationary phase
To evaluate the application of solubility parameters to bonded stationary phases the distribution constant can be calculated from Eq.1-9 and by rearranging Eq. 1-7 V can be evaluated. This was done for several of
the columns used for this work and in each case, no consistent V value s
was obtained. The major drawback lies in obtaining a valid solubility parameter for the stationary phase (6^). It must be remembered that the stationary phase consists of a monolayer of bonded material, which may not have the same properties as the bulk material, unreacted silanol groups and organic modifier from the mobile phase. It would appear then that a AG value cannot be obtained experimentally unless one is able to obtain an accurate V value.
For bonded phases AG cannot be calculated directly because no accurate K or values can be measured. Since no independent measure
ment for AS can be made, equation 1-1 cannot be solved. It is possible however, to obtain accurate AAG'values as shown in equations 1-10 through 1-13.
AG^ = -RT In k'^ - RT In <!> (1-10)
AG; - AG„ = RT In k' - RT In k' (l-ll)
A B B A
AAG' „ = RT In a (1-12)
" " k\ (1-13)
The only assumption made is that the phase ratio ((^) is the same for both solutes. This is valid for molecules of similar size. The AAG' values allow one to evaluate the contribution of different substituents on the solute molecule to the overall retention behavior.
Since only AAG'values can be calculated then only relative
changes in entropy can be calculated because equation 1-1 must be used to arrive at a AS value. By combining equations .1-1 and 1-10 a AAS' value can be obtained (Eq. 1-14).
AAS' ^ - R In ct (1-14)
The chromatographic experiments are used to obtain information about the chemical and physical nature of the bonded phase. The reten
tion volume or peak position under specific chromatographic conditions provide information about the strength of the interaction between the solute and the stationary phase, the capacity and the selectivity. The peak broadening gives information about the efficiency and the differ
ence in the interaction between the various probes used.
25 Peak Position
For this work all elution chromatography, except as so noted, is in the linear range. This means that all peaks are Gaussian in shape and the distribution constant (K) is independent of. sample size.
The basic retention parameter is the retention volume, V_. This IV
is the volume of mobile phase that is necessary to elute the solute to the peak maximum (45). It can be calculated very easily from Eq.1-15, where t = retention time and
= t^ • F/R (1-15)
F/R = flow rate of the mobile phase. F/R is usually given in milliliters per minute and t in seconds. V can also be used to calculate the
distribution coefficient (Eq. 1-16) if the volume of the stationary, phase (V^) for a liquid-liquid partitioning, or the area of the stationary
phase for a liquid-solid adsorption is known.
It must again be pointed out that V or A for bonded phases is difficult
to measure accurately, therefore an accurate K value cannot be obtained.
Equation 1-16 assumes that the retention is due to only one mechanism, either partitioning or adsorption. It is possible however, that on a bonded phase both these processes as well as exclusion can be involved during the chromatographic process. Equation 1-16 must
therefore be expanded to Equation 1-17 to include all three of these mechanisms.
26 V„ = V„ + KV + K'A + K' 'V, (1-17)
R M s s i
= Interstitial volume.
If one mechanism predominates the other two can usually be ignored.
However, data to be presented in this work will show that both mechan
isms can and do exist. Furthermore, bonded phases that have small pore sizes, use trifunctional modifiers, and are subsequently capped with a trimethylchlorosilane can have very non-uniform surfaces.
Clusters of polymer-like chains and single strands spaced further apart may exist on these stationary phases as well as smaller
pores which exclude the bonded phase. Equation 1-17 can be further expanded to take this into account. On areas of the stationary phase where the density of coverage is different or where the chain length is shorter (because of capping) the distribution constant for a solute is going to change.
'e - 'M + Vs---'
+ (K^"V^ + K2"V^ + ...)
At the present time there is considerable debate over the reten
tion mechanisms of bonded reversed phases. There are those who argue that the retention mechanism is a function of the surface area of the total bonded phase (46). While this may be true for some solvent systems which cannot solvate the bonded hydrocarbon, data presented in this work and others ( 8 ) show that the stationary phase is modified by the organic component of the mobile phase and that the overall retention mechanism is a function of the type and number of molecules
27 bonded to the surface as well as the organic modifier used in the mobile phase.
The efficiency of a chromatographic column is usually described in terms of the number of theoretical plates, or the height equivalent to a theoretical plate. The terms originate from the model by Martin and Synge (47). The values for the number of theoretical plates can be calculated from several equations (44 ). One of the more commonly used formulae is Equation 1-19,
N = 5.54 (1-19)
N = number of theoretical plates t^ = retention time
Wi/2 = width of the peak at half height
The height equivalent of a theoretical plate (HETP) can be obtained by dividing the length of the column (N) by the number of theoretical plates (Eq.1-20).
H or HETP = L/N ( 1-20)
The major contributions to H are summarized in Equation 1-21.
^ \ «SM
HL = broadening due to longitudinal diffusion
Hg = broadening due to stationary phase mass transfer effect
= broadening due to mobile phase effects
= broadening due to diffusion or mass transfer across the stagnant mobile phase
These contributions to band broadening can be grouped into three areas.
The first is or diffusion of the solute in the direction of the flow in the mobile phase. (Eq. 1-22) is only significant at slow flow rates and in mobile phases where diffusion is rapid. In liquid
chromatography is normally assumed to be zero. The second is broad
ening due to mobile phase effects, (Eq. 1-23). consists of an eddy diffusion term (H^,) (Eq. 1-24) and diffusion effects (H^) (Eq. 1- 25). Again, because of the high linear velocities in liquid
chromatography and the large diffusion coefficients, is small and which is velocity independent dominates. The third portion is the sum of the contribution of the band broadening due to mass transfer in the stationary phase (Hg) (Eq. 1-26) and mass transfer through tht stagnant mobile phase (Hg^) (Eq. 1-27).
^ 9 V Dm (1-22)
Y = obstruction factor due to packing
Dm = solute diffusion coefficient in the mobile phase V = linear velocity of the mobile phase
+ Hp (1-23)
Hp = dp (1-24)
A = a function of the packing structure dp = particle diameter
H„ - ^ a-25,
= a function of the packing structure
H, = 5-kLA^ a-26)
" D tt+t')"' s
q = geometric factor
= diffusivity of the solute into the stationary phase
. (1-* •<- a-27)
<j) = the fraction of '.the total mobile in the intra- particle space
Y = tortuosity factor inside the particle
This information can be obtained experimentally by a plot of H vs V. This is known as a van Deempter (48) plot and Eq. 1-21 can be expressed in a form known as the van Deempter equation (Eq. 1-28).
H = A + B/v + Cv (1-28)
The A term of the van Deempter equation is the flow independent or
eddy diffusion term (H-^ • This is dependent upon stationary phase particle size. The B or longitudinal diffusion term (H^) is not important in
liquid chromatography. The C term is velocity dependent and is the sum of the mass transfer terms in both phases (H_ + H ). It is this last
30 term which is of most interest. The C term tells us if all the solute molecules encounter the same type of stationary phase under the condi
tion of the experiments.
The non-chromatographic techniques that were used to char
acterize the bonded phases were Nuclear Magnetic Resonance Spectrometry, batch extraction experiments, and elemental analysis.
Carbon 13 NMR was used to investigate the solvent bonded phase interaction. While NMR is more commonly used to give structural infor
mation, it can also provide information about molecular motion (49).
With 13 C NMR, for which the chemical shifts are much larger than for
protons and the intemuclear dipolar broadening much less, it has become possible to use this technique for obtaining information about the molecular motion of bonded species. The major disadvantage of 13 C NMR is the low natural abundance of 13 C. This was overcome by the use
of Fourier Transform methodology and by using the 10 pm bonded phases which have a high packing density.
In addition to information provided by the chemical shift of the atoms due to their differing chemical environments, one can also use the broadening of. the signal to gain information .about the physical nature of the molecular species. The broadening of the signal can be caused by chemical shift anisotropy or by short relaxation times, both of which are due to restricted molecular motion. In solids, the chemical shift anisotropy causes line widths which are significantly
31 broader than in liquids (50 )„ It has been shown (51' ) that for
adsorbed molecules the signal may be significantly narrowed by an
increase in the molecular motion of the adsorbed species relative to the true solid. Chemisorbed species have also been studied and similar motional narrowing has been observed (52 ). Thus the width of the 13 C
NMR signal may be used as a qualitative indicator of the molecular motion of a bonded phase. If the bonded phase is highly solvated, then one would expect narrower peaks than for a bonded phase that is not solvated. An analogy would be the branches of a bush. If the branches were intertwined (non-solvated system), then they would have little motion in a wind; but if each branch was attached only at the stem (solvated system) then they would have a significant freedom of motion in a wind.
Batch Extraction Experiments
A comparison of the bonded phase used in liquid chromatography to liquid-liquid extraction was carried out. These experiments were performed to provide information as to how much of the organic modifier is adsorbed by the bonded phase. Two types of experiments were per
formed. In one, the organic phase was a bulk hydrocarbon; in the other, the actual bonded supports were used as the organic phase. In each case the "aqueous layer" was a mixture of water and an organic modifier such as methanol or tetrahydrofuran.
Materials and Reagents
All columns were 1/4" OD 316 stainless steel with Parker or Swagelol^ end fittings. Stainless steel frits of 2.0 pm pore size were used to keep the packing material in place and exclude contaminant particles. The internal dimensions of the columns were 2.1 mm ID X 250 mm except the fatty acid amide, which was 3 mm ID x 200 mm..
The silica which was used for the Grignard and the silane reac- tions was Spherisorb , a 10 ym spherical totally porous silica obtained from Spectra-Physics, Santa Clara,. California. The 5% CDS bonded phase was the 10 ym Spherisorb particles modified with octadecyltrichloro- silane. It was also obtained from Spectra-Physics. The 10% ODS bonded phase was an irregular shaped silica particle modified with octadecyl- trichlorosilane and capped with trimethylchlorosilane. This was
supplied by Waters, Inc., Waltham, Massachusetts. The particle size of the ]x Bondapal^ was 10 Pm. The remaining bonded phases were obtained from EM Laboratories. They were all irregular shaped silica particles (Lichrosorb) of 10 ym diameter that had been modified with octadecyldi- methylchlorosilane (RP-18), octyldimethylchlorosilane (RP-8),
ethyldimethylchlorosilane (RP-2) and triethoxy-y-propylamine (NH2). The fatty acid amide column was made by further derivatizing the NH2 bonded phase with 9,12,15 octadecatrienoic (linolenic) acid.
The phenyl bonded phase was made by modifying the Spherisorb with trichlorophenylsilane obtained from PGR Research Chemicals, Inc.
A complete description of the physical characteristics of these phases is given in Table 2.1.
A method similar to the one described by Little et al. (53) was used for the phenyl bonded phase. Approximately 1.5 gms of 10 pm Spherisorb was placed in a 25 ml flask that had previously been silanized with trichloromethylsilane ( PGR Research Chemicals, Inc.) The
silica was covered with 10 ml of dichloromethane (Mallinkrodt Inc., AR grade redistilled and dried over sodium). Then, 1.5 ml of trichloro
phenylsilane (Aldrich Chemical Company) was added. The
mixture was covered and stirred using ultrasonification for 30 minutes and then was allowed to further react at room temperature for an addi
tional two hours. The solvent and excess silane were evaporated in a drying oven at 55° C. The beads were washed on a Millipor^LS type filter under suction with hexane, tetrahydrofuran, methanol, water and acetone. The beads were dried again overnight in a 55° C oven and then stored in a dessicator.
A butyltrichlorosilane and a dodecyltrichlorosilane bonded phase were prepared by a variation of the above described method. A procedure described by Gilpin (19) was used. 1.5 gms of Spherisorb were dried for 24 hours prior to modification at 150° G under a flow of dry Argon.
Table 2.1. Bonded phase specifications
Surface Functional Manuf.
area Pore Length % Carbon group % Calc. %
Before Mod Size of chain bonded derlvitlzation derlvitlzation Spherlsorb
5% ODS pbondapak 10% ODS
200 m /gm 80-100A
300-350 m /gm
capped with C,
Merk 20% ODS RP-18
Amide Before Mod After Mod Phenyl
105 m /gm 150A C^g
250 m /gm lOOA
250 m /gm lOOA
200 m /gm BO-IOOA Phenyl group
CHq t R-Si-Cl
I ^ R-Sl-Cl
35 The silica was transferred to a previously silanized flask and covered with 10 ml of dried redistilled toluene. 1.5 ml of the silane
(butyltrichloro or dodecyltrichloro) was added to the flask. The
mixture was refluxed overnight and filtered the next day, using the same solvents described above. The beads were then dried in an oven at 100° C for several hours and stored in a desiccator.
This reaction was used to prepare a bonded phase that had a long hydrocarbon chain with some functional groups incorporated into it.
Lichrosorb NH2 (10 um) bonded phase was dried at 100° C for 24 hours prior to use. 1.5 gms of this material were put into a reaction
flask and covered with dried hexane. A 100% (approx. 1 ml) stoichio
metric excess of linolenic acid (9,12,15 octadecatrienoic acid) was added and the mixture was refluxed overnight. The beads were then washed with hexane, tetrahydrofuran, methanol, water and acetone. They were dried again at 100° C overnight and stored in a desiccator.
The Grignard reaction procedures that were used are similar to those described by Locke, Schmermund and Banner G7)> Approximately 1.5 Spherisorb 10 pm silica were placed in the glass apparatus shown in Fig.2.1. All inner surfaces of the glass had been deactivated with tri- methylchlorosilane. A heating mantle was placed around the glass tube and heated to 150° C. The actual temperature of the beads was measured by a thermocouple inserted through the upper stopcock. Dry Argon was
GLASS DISC- 2 m PORE SIZE
TO ARGON TANK STOPPER
Figure 2,1. Apparatus for drying silica beads
passed through the beads for three to four hours prior to the chlorina- tion reaction. The glass apparatus was then inverted, causing the beads to fall into the round bottomed flask. Redistilled thionyl chloride was introduced into the flask to chlorinate the surface hydroxyl groups of the silica. The silica was allowed to react for two hours with reflux and stirring. The excess thionyl chloride was then evaporated with a stream of dry nitrogen. The flask was warmed to prevent the condensa
tion of water. The beads were covered with dry, distilled THF or diethyl ether while the organomagnesium halide was being prepared. This was done by adding about 0.5 gms of magnesium turnings to approximately 20 ml of dry, distilled THF or diethyl ether. About 2 ml of the desired organohalide was then added to the flask. Gentle warming was usually required to initiate the reaction. When the reaction was completed, this mixture was added to the dry chlorinated silica and allowed to reflux overnight. The beads were filtered to remove the excess solvent and washed with water (slightly acidic), THF, hexane and acetone. They were then dried at 100° C and stored in a desiccator. Table 2.2 lists the bonded phases that were prepared by this method.
Column Packing Procedure
Since all bonded phase particles had diameters of 10 vim, it was necessary to use a slurry packing method.
1.2 gm of the packing material were suspended in 12 ml of a 50/50 mixture by volume of 1,1,2,2-tetrabromoethane and 1-butanol.
Ultrasonic stirring was used to assure complete dispersion of the
38 Table 2.2. Bonded phases prepared by Grlgnard reactions
Bonded Molecule Parent Silica % by wt C
Octane Porasil 60 0.85
Octane Porasil 400 5.10
Octane Spherisorb 2.37
Pentene Spherisorb 1.61
Octane Spherisorb 1.20
bonded phase in the solvent mixture. The suspension was prepared
several hours prior to the packing and stirred several times during this period to assure complete dispersal and solvation of the beads by the solvents. Immediately prior to pouring the beads into the reservoir column, they were again stirred in the ultrasonic bath. A Haskell pneumatic aniplification pump (model DST-150A) with a 50/50 hexane- chloroform solvent mixture was used to pack the analytical column. The pressure was maintained at 10,000 psi until all the suspension solvents had been pumped through the column. The packed columns were then washed with THF and methanol to remove the hexane-chloroform mixture and stored in methanol until they were used.
All solvents used for this procedure were analytical reagent grade. The hexane, chloroform, THF and methanol were filtered through
.45 ym pore size Millipore filters prior to use.
Methyl Red Experiment
Methyl Red has been used to measure the surface area of
silica (54)^ The dye will be adsorbed from a solution onto the surface of the silica presumably by interactions with the silanols. By
measuring the amount of dye that has been taken out of solution and by knowing its surface area the surface are of the silica can be
measured. This experiment was performed with the bonded phase to deter
mine the number and the accessi'bility of the residual silanol groups.
0.0131 gms of methyl red were dissolved in 1 liter of benzene. The absorption of this solution was measured at 521 nm. The bonded phases were shaken in 5 ml aliquots of this solution for 2.5 hours. A portion
40 of the supernatant was withdrawn and its absorbance was again measured at 521 nm. By using a molar absorptivity value of 5.75 x 10 for the 4
methyl red, the amount of the dye adsorbed by the silica could be cal
The 13 C NMR spectra were obtained using a Bruker WH-90 spectrom
eter operating at 22.62 MHz. The spectrometer was operated in the pulse mode with a pulse length of 12 psec, and the spectra were broad band decoupled. The Fourier Transform of 280,000 scans (an overnight run) was accomplished using a Nicolet 1080 Data System. A "Bruker variable
temperature probe allowed spectra to be obtained at elevated temperatures.
About one gram of the bonded material was used in the 10 ram ID NMR tubes.
All organic solvents were AR grade (Mallinckrodt or Fisher) and were filtered through .45 pm pore size Millipore filters. When only organic
solvents were used, the lock material was deuterochloroform (Aldrich).
When mixtures of organic and aqueous solvents were used, deuterium oxide (Stohler Isotope Chemicals) which was used instead of water, also served
as the lock material. For the non-solvated spectra, a sealed coaxial tube containing deuterium oxide was used for the lock.
Batch Extraction Experiments
The batch extraction experiments were perfomed using heptane (J. T. Baker, AR grade) as the bulk hydrocarbon phase and a 50/50
mixture of water (distilled over KMNO^) and methanol, THF, dioxane, acetonitrile or ethanol (Fisher) in the aqueous phase. The composition
41 of the two phases was analyzed by gas chromotography. A gas chromatograph with a thermal conductivity detector and a Porapak Q column at 110° C (195° C for heptane) was used. The injection port temperature was set at 250° C and helium (reactor grade) at a flow rate of 60 ml/min was used as the carrier gas. A Spectra-Physics Autolab System I integrator was used to measure the peak area ratios and the retention times. All runs were done in triplicate.
The batch experiments performed with the bonded phases were similar to those described above. The bonded phases were used instead of the bulk hydrocarbon (heptane). The composition of the liquid phase was analyzed on an Envirotech Model 15C3 gas chromatograph with a thermal conductivity detector. Reactor grade helium at a flow rate of 40 ml/min through a Porapak Q & R (50/50) at a temperature of 180° C was used for the analysis. A Spectra-Physics Autolab System I integrator was used for area ratio measurements. Five replicate injections were used for each analysis.
The purpose of the batch extraction experiments with heptane and the "mobile phase" (water plus the various organic modifiers) was to see how the organic modifier distributes itself between the two phases.
For the second part which involved the bonded phases it was possible to determine how much of the organic modifier was extracted into the stationary phase.
Liquid Chromatographic Experiments
The peak position on thermod3nQamic studies were performed on a Spectra-Physics 3500 B dual reciprocating pump high performance liquid
42 chromatograph with a Spectra-Physics model 235 UV detector set at 254 iim. Retention times were measured by a Spectra-Physics Autolab System I integrator. The column temperature was maintained by a Haake model FE circulating bath which circulated water at the desired temperature through a jacket which contained the colimin. Sample sizes were 10 yl.
The concentration of the sample molecules was approximately 0.1% by volume in methanol. The water was distilled over KMnO^ and filtered through a .45 Mm pore size Millipore filter prior to use. The organic solvents were analytical reagent grade also filtered through a .45 pm pore size Millipore filter prior to use. The tetrahydrofuran was dis
tilled over KOH prior to filtering. All solvents were degassed before use.
The kinetic or peak broadening studies were performed on a Varian model 5000 high performance liquid chromatograph. The column temperature was maintained by a heating block attached to the instrument.
The same procedure as described was used for solvent purification.
However, it was not necessary to degas the solvents for this instnnnent.
Sample sizes and concentrations were the same as described above.
Elemental analysis was performed on the bonded supports for carbon by Chemalytics Inc. (Tempe, Az.) or the University Analytical Center at the University of Arizona.
According to Kiselev's classification system [Klselev and Yaskln 1969 (22)] only non-specific interactions are encountered on Type I surfaces. For a bonded silica to be considered a Type I, all the
43 available silanols would have to be covered. For most HPLC bonded
phases the calculated average percentage coverage (based on manu
facturer's information) is between 20% and 75%. This allows specific interactions to take place if the probe molecule can successfully compete with the solvent molecules for the remaining silanol sites.
Therefore, one must consider both specific and non-specific interactions.
During this study, benzene and alkylbenzene derivatives always gave symmetrical peaks but the strong hydrogen bonders such as aniline pro
duced severe tailing even on the most highly derivatized packing materials, materials.
The choice of solute molecules to be used as molecular probes with which to characterize the bonded phases involved consideration of the tjrpe of interactions available as well as consideration of the sensitivity of the detection system. All of the probe molecules had to have chromophores which would absorb light at 254 nm. For this reason benzene, toluene, ethyl benzene and isopropyl benzene were used to look at non-specific interactions while phenol, benzyl alcohol, acetophenone and aniline were chosen as specific interacting molecules.
Bonded Phases Studied
The bonded phases that were used in this study are those which showed reasonable retention characteristics for the probe molecules used. Although a number of bonded phases were made with the Grignard reaction, none was used in this study. As can be seen in Table 2.1 only one, the Porasil c(^400, had a significant amount of carbon bonded to it. This material, however, was of large particle and pore size
(400 A) which gives it a low surface area and therefore very poor efficiency. In fact, the large pore size may have contributed to the amount of carbon that was bonded to this silica. Other workers (.55) have used silicas modified with low amounts of carbon but they do not make particularly good reversed phase supports.
Of the trichlorosilane derivatized silicas, only the phenyl bonded material was fully characterized. The remainder of the packing materials used are commercially available. Table 2.1 describes these phases. There were two more commercial phases which were not fully characterized because of their poor retention characteristics. The Lichrosorb NH2 is, according to the manufacturer's literature, designed for separation of polar compounds. It was not able to separate the alkyl benzenes. The Lichrosorb RP-2 was able to separate the alkyl benzenes, but only with the poorest of resolution at room temperature.
At elevated temperatures the solutes eluted with the solvent front.
Percent by weight carbon is usually used as an indication of how hydrophobic the surface of a modified silica is. While it is certainly necessary to know this number, one also needs to know the chemical formula of the bonded material as well as the surface area of the parent silica gel. An estimate of the surface area of the silica is usually readily obtainable from the manufacturer's literature. The nitrogen BET method (56) is used almost exclusively to obtain this Information. It is also necessary to know the complete formula of the bonded material not merely the chain length of the carbon moiety if mono- or di-chloro silanes are used. The E.M. Laboratories Lichrosorb